Study of the Effect of Absorbed Cu Species on the Surface of Specularite (0 0 1) by the DFT Calculations

Study of the Effect of Absorbed Cu Species on the Surface of Specularite (0 0 1) by the DFT Calculations. Abstract: Cu 2+ exhibited a good activation effect on specularite. However, its microscopic activation mechanism needs further study. Additionally, Cu 2+ was mainly present in the ﬂotation solution as Cu 2+ , Cu(OH) + , and Cu(OH) 2 at pH = 7. Therefore, density functional theory (DFT) calculations were used to investigate the effect of Cu species such as Cu 2+ , Cu(OH) + , and Cu(OH) 2 adsorbed on the crystal structure and properties of the specularite (0 0 1) surface. The adsorption mechanism of different Cu components on the surface was also further clariﬁed by the analyses of the adsorption model, adsorption energy, partial density of states (PDOS), charge transfer, and bond properties. In addition, the obtained results are discussed. Based on the obtained results, it can be concluded that the geometric structure and electronic properties on the surface changed after adsorbing Cu components and that the O3–Fe1–O1 structure was more susceptible to the adsorbates. The adsorption engines results show that Cu components could be spontaneously adsorbed onto the specularite (0 0 1) surface with adsorption energies of − 0.76, − 0.85, and − 1.78 eV, corresponding to Cu 2+ , CuOH + , and Cu(OH) 2 , respectively. Therefore, the adsorption stability of the Cu species on the specularite surface increased in the order of Cu 2+ < Cu(OH) + < Cu(OH) 2 . Additionally, the adsorption sites for Cu species on the surface were different. Cu 2+ interacted mainly with O atoms on the surface, forming Cu–O complexes, while Cu(OH) + and Cu(OH) 2 acted mainly through the O atom of –OH, interacting with Fe atoms to form Cu–O–Fe complexes. The formation of Cu–O and Cu–O–Fe complexes increased the adsorption sites for sodium oleate, with more hydrophobic species being generated to improve the ﬂoatability of specularite. specularite (0 0 1) surface the PDOS of the Cu atom near the Fermi level was contributed by the 4s, 2p, and 3d orbitals, in which the contributions of Cu 3d and 4s orbitals were strong, and that played an important role in the reactivity of Cu 2+ adsorbed on the surface of specularite. Combined with the PDOS of Fe1 and O1 atoms on the surface of specularite (Figures 3b and 5a), it can be observed that the PDOS of the Cu 3d orbital peak at − 1.3 eV and the Cu 2p orbital at 5 eV overlapped with the 2p orbital of the O1 atom on the specularite surface, indicating that Cu 2+ mainly interacted with the O atoms on the surface of the specularite.


Introduction
Copper ions are often used as an activating ion in flotation to increase the floatability of minerals, and there were many studies on the activation mechanisms of copper ions on metallic sulfide minerals (e.g., sphalerite and pyrite) and nonmetallic oxidized ore (e.g., chlorite and quartz) [1][2][3]. Scholars [4,5] analyzed the hydrolysis products of Cu 2+ in different pH ranges by solution chemistry calculations. Cu 2+ could be hydrolyzed in the aqueous solution with the change of pH to form five components: Cu 2+ , Cu(OH) + , Cu(OH) 2 , Cu(OH) 3 − , and Cu(OH) 4 2− . At pH less than 7.0, Cu 2+ was the predominant species, and CuOH + and Cu(OH) 2 became the main species at pH of 7.0-10.7, while at pH greater than 10.7, the copper species in the solution were mainly in the form of Cu(OH) 2 , Cu(OH) 3 − , and Cu(OH) 4 2− . Flotation is one of the most common methods used to recover iron ore, which includes reverse flotation of gangue with cationic collector [6][7][8] and direct flotation of iron ore with anionic collector [9][10][11]. Compared with reverse flotation, direct flotation of iron ore The convergence tolerances were set as follows: energy tolerance, 2 × 10 −5 eV/atom; maximum force tolerance, 0.05 eV/Å; maximum displacement tolerance, 0.002 Å; maximum stress, 0.1 GPa; SCF tolerance, 1 × 10 −6 eV/atom. If there was no special explanation, all parameter settings were consistent during the calculation process.
First, the original unit cell of specularite was constructed. The unit cell parameters were a = b = 5.03 Å, c = 13.75 Å, α = β = 90 • , and γ = 120 • . Li et al. [27] studied the surface energy of several specularite crystal surfaces through DFT calculations, and the results showed that the (0 0 1) surface of specularite has the lowest surface energy. Therefore, the (0 0 1) surface was constructed according to the overall structure of specularite. A 2 × 2 × 1 supercell with 12 atomic layers was used for the simulation. The vacuum-layer thickness was set to 40 Å to avoid the interaction between the surface structure layers as well as to eliminate the effect of periodicity. The optimal surface structure was obtained by optimizing the geometry of the supercell, as shown in Figure 1. Then, the optimized Cu species were placed on the surface of the model, and their interaction was simulated.
Minerals 2021, 11, x FOR PEER REVIEW 3 of 16 BFGS algorithm to optimize the structure of the model [26]. The cutoff energy was 400 eV. The convergence tolerances were set as follows: energy tolerance, 2 × 10 −5 eV/atom; maximum force tolerance, 0.05 eV/Å ; maximum displacement tolerance, 0.002 Å ; maximum stress, 0.1 GPa; SCF tolerance, 1 × 10 −6 eV/atom. If there was no special explanation, all parameter settings were consistent during the calculation process. First, the original unit cell of specularite was constructed. The unit cell parameters were a = b = 5.03 Å , c = 13.75 Å , α = β = 90°, and γ = 120°. Li et al. [27] studied the surface energy of several specularite crystal surfaces through DFT calculations, and the results showed that the (0 0 1) surface of specularite has the lowest surface energy. Therefore, the (0 0 1) surface was constructed according to the overall structure of specularite. A 2 × 2 × 1 supercell with 12 atomic layers was used for the simulation. The vacuum-layer thickness was set to 40 Å to avoid the interaction between the surface structure layers as well as to eliminate the effect of periodicity. The optimal surface structure was obtained by optimizing the geometry of the supercell, as shown in Figure 1. Then, the optimized Cu species were placed on the surface of the model, and their interaction was simulated. The stability of adsorbates surface could be determined using the adsorption energies (Eads) [28], and the adsorption energy of the adsorbates on the specularite surface was calculated as follows [29][30][31]: where E ads represents the adsorption energy; E adsorbate/slab represents the energy of the adsorbed specularite (0 0 1) surface; E adsorbate represents the energy of the adsorbate; and E slab represents the energy of the specularite (0 0 1) surface. The more negative the adsorption energy, the stronger the interaction between the adsorbates and the specularite surface [32,33].

The Effect of Cu Species Adsorbed on the Structure of the Specularite (0 0 1) Surface
Copper ions were hydrolyzed into different species in an aqueous solution as a function of pH. Previous studies [12] had shown that specularite modified with Cu 2+ has better floatability. In addition, Cu 2+ , Cu(OH) + , and Cu(OH)2 were the main species of copper ions in flotation pulp under pH = 7. Therefore, the adsorption models of three Cu components The stability of adsorbates surface could be determined using the adsorption energies (E ads ) [25], and the adsorption energy of the adsorbates on the specularite surface was calculated as follows [28][29][30]: where E ads represents the adsorption energy; E adsorbate/slab represents the energy of the adsorbed specularite (0 0 1) surface; E adsorbate represents the energy of the adsorbate; and E slab represents the energy of the specularite (0 0 1) surface. The more negative the adsorption energy, the stronger the interaction between the adsorbates and the specularite surface [31,32].

The Effect of Cu Species Adsorption on the Electronic Properties of Specularite
To understand the effect of Cu 2+ adsorption on the surface electronic properties of specularite, the PDOS of the Fe and O atoms on original and Cu-modified specularite surface were analyzed. The results show that the PDOS of surface atoms changed after Cu species adsorbed on the specularite (0 0 1) surface. Figure 3 shows the PDOS of Fe1 atom on specularite (0 0 1) surface before and after treatment with Cu 2+ . The black dotted line at 0 eV in the figure represents the Fermi level. The valence electron configuration of the Fe atom was Fe 3d 6 4s 2 . The PDOS of Fe atom was composed of 4s, 3p, and 3d orbitals, and the PDOS of Fermi level was mainly contributed by the Fe 3d orbital. Compared with the results before Cu 2+ adsorption (Figure 3a), the PDOS of Fe atom changed significantly after Cu components adsorbed on the surface of the specularite. After Cu 2+ component adsorbed on the specularite surface (Figure 3b), the PDOS of Fe 3d orbital on the surface decreased, and a new Fe 3d orbital peak appeared at about −2 eV, while the PDOS of Fe 3p orbital decreased. After Cu(OH) + adsorbed on the specularite surface (Figure 3c), the peak of Fe 3d orbital increased strongly. Similarly, the number of Fe 3d orbital peaks also increased to a certain extent. However, the PDOS peak of Fe 3d orbital disappeared after 4 eV. Although the PDOS peak of Fe 4s orbital increased, its peak near the Fermi level disappeared, which indicates that the contribution of Fe 4s orbital to Fe atom activity was reduced. It is noteworthy that the two new PDOS peaks of the Fe 4s orbital and a new PDOS peak of the Fe 3d orbital appeared at around -20 eV. This may have been caused by the interaction between the Fe atom on the surface of specularite and the Cu(OH) + component. After Cu(OH) 2 adsorbed on the surface of specularite (Figure 3d), the PDOS of the Fe 3d orbital disappeared after 4 eV. The PDOS of the 4s orbital increased, but its PDOS peak near the Fermi level disappeared, indicating that the contribution of the 4s orbital to the activity of Fe atoms decreased. It is worth noting that the PDOS of Fe 4s and Fe 3d orbitals each added a new peak at around -20 eV, which may have been caused by the interaction of the Fe atom on the surface of the specularite and Cu(OH) 2 component.
The adsorption of Cu species on the surface of specularite can also cause changes in the PDOS of O atoms. Therefore, the changes in the PDOS of O atom on the surface before and after the adsorption of Cu components on the specularite surface were studied ( Figure 4). The valence electron configuration of O was 2s 2 2p 4 , which indicates that the PDOS of the O atom was composed of 2s and 2p orbitals. As shown in Figure 4, the PDOS of O 2s orbital made little contribution to the reactivity of the O atom on the surface that was far from the Fermi level, and the PDOS vicinity of the Fermi level was mainly contributed by the O 2p orbital. Compared with the PDOS before the Cu components adsorbed, the position of the O atom PDOS peak did not move significantly, but the peak intensity had a certain change. In particular, the PDOS of the O atom changed most obviously after the Cu 2+ component adsorbed on the specularite (0 0 1) surface. After Cu 2+ adsorbed on the surface of the specularite (Figure 4b), the PDOS peak intensity of the O 2s orbital on the surface was significantly reduced, and the PDOS peak intensity of O 2p orbital was significantly enhanced, especially the PDOS peak at −2 eV. After Cu(OH) + and Cu(OH) 2 adsorbed on the specularite surface (Figure 4c,d), the PDOS of the O 2s orbital and the O 2p orbital changed little. These indicate that there was a strong interaction between the O atoms on the surface of the specularite and the Cu 2+ component, but its adsorption of Cu(OH) + and Cu(OH) 2 showed weak reactivity.   Figure 4, the PDOS of O 2 orbital made little contribution to the reactivity of the O atom on the surface that was fa from the Fermi level, and the PDOS vicinity of the Fermi level was mainly contributed b the O 2p orbital. Compared with the PDOS before the Cu components adsorbed, the po sition of the O atom PDOS peak did not move significantly, but the peak intensity had    Table 3. When Cu 2+ was placed on the (0 0 1) surface of the specularite (as shown in Figure  2b), the distances between the Cu atoms and Fe1 and O1 atoms on the specularite surface were 1.614 Å and 1.613 Å , respectively. After geometric optimization, the distance be-   When Cu 2+ was placed on the (0 0 1) surface of the specularite (as shown in Figure 2b), the distances between the Cu atoms and Fe1 and O1 atoms on the specularite surface were 1.614 Å and 1.613 Å, respectively. After geometric optimization, the distance between Cu and O1 atoms on the surface increased to 1.987 Å, but it was smaller than the sum of the radii of Cu and O atoms. When the distance between two atoms was close to or less than the sum of their atomic radii, a chemical bond was formed between these atoms [33,34], indicating that Cu atoms and O1 atoms on the surface may form Cu-O chemical bonds. Among them, the distance between Cu and Fe1 atoms increased to 2.387 Å, which was larger than the distance between Cu and O1 atoms, indicating that the O atoms on the surface of specularite (0 0 1) had a stronger adsorption effect on Cu 2+ and that the adsorption of Cu 2+ on the specularite surface was mainly through Cu atom bonding with O1 atoms on the surface. The adsorption energy of Cu 2+ on the surface of specularite was calculated to be −0.76 eV, and a negative value indicates that the adsorption of Cu 2+ component on the (0 0 1) surface of specularite was spontaneous.
When Cu(OH) + was placed on the specularite (0 0 1) surface (as shown in Figure 2c), the distances between the Cu atoms of Cu(OH) + and the Fe1 and O1 atoms on the specularite surface were 1.665 Å and 1.661 Å, respectively, and the distance between OI atom of Cu(OH) + and Fe1 atoms on the specularite surface was 1.538 Å. After geometric optimization, the bond length between the Cu atom and the surface O1 atom increased to 1.930 Å, but it was less than the sum of the radii of the Cu and the O atoms, indicating that the Cu atom might have formed a chemical bond with the surface O1 atom. The distance between Cu and Fe1 atoms increased to 2.675 Å, which was significantly larger than the bond length of Cu-O, indicating that the oxygen atoms on the specularite surface (0 0 1) had a stronger adsorption effect on Cu atoms of Cu(OH) + . At the same time, the distance between OI atoms of Cu(OH) + and Fe1 atoms on the specularite surface changed from 1.538 Å to 1.876 Å after optimization, which was smaller than the sum of the radii of Fe and O atoms. It shows that the adsorption of Cu(OH) + on the surface was achieved not only by the bonding of Cu atoms in the Cu(OH) + component with the surface O1 atoms but also by the bonding of OI atoms with the surface Fe atoms. The adsorption energy of Cu(OH) + on the specularite surface was calculated to be −0.85 eV. A negative value indicates that the adsorption of Cu(OH) + on the (0 0 1) surface of specularite was spontaneous.
When Cu(OH) 2 was placed on the specularite (0 0 1) surface (as shown in Figure 2d), the distances between Cu atoms of Cu (OH) 2 and Fe1 and O1 atoms on the surface of specularite were 1.708 Å and 1.713 Å, respectively. In addition, the distance between OI atoms of Cu(OH) 2 and Fe1 atoms on the surface of specularite was 1.712 Å, and the distance between OII atoms and Fe5 atoms on the surface of specularite was 2.296 Å. After geometric optimization, the distances between the Cu atom of Cu(OH) 2 and the surface O1 and Fe1 atoms increased to 2.146 Å and 2.750 Å, respectively. The distance between the Cu atom and the O1 atom was greater than the sum of its atomic radii, indicating that the Cu atom of Cu(OH) 2 did not form a chemical bond with the surface O1 atom. While the distance between the OI atom of Cu(OH) 2 and the Fe1 atom on the specularite surface changed from 1.721 Å to 1.887 Å, and the distance between the OII atom and the Fe5 on the specularite surface had been reduced from 2.296 Å to 1.909 Å, both of which were smaller than the sum of the radii of Fe and O atoms, indicating that the adsorption of Cu(OH) 2 on the specularite surface was mainly achieved by the bonding of OI and OII atoms of the Cu(OH) 2 component with Fe1 and Fe5 on the specularite surface, respectively. The adsorption energy of Cu(OH) 2 on the surface of specularite was calculated to be -1.78 eV. A negative value indicates that the adsorption of Cu(OH) 2 on the specularite(0 0 1) surface was spontaneous.
The more negative the adsorption energy is, the stronger the adsorption capacity of the adsorbate on the mineral surface is [35][36][37]. Comparing the adsorption energy of Cu components on the surface of specularite, the results show that the adsorption energy of Cu(OH) 2 component on the specularite (0 0 1) surface was the largest, followed by CuOH + and Cu 2+ . Therefore, the adsorption stability of Cu species on the surface of specularite increased in the order of Cu 2+ < Cu(OH) + < Cu(OH) 2 .

Density of States Analysis of Interaction between Cu Species and Specularite (0 0 1) Surface
In order to further verify the interaction of Cu 2+ , CuOH + , and Cu(OH) 2 on the surface of specularite, the partial density of states (PDOS) of atoms of Cu components are shown in Figure 5. As shown in Figure 5, the PDOS of Cu atoms after adsorption on the specularite surface was composed of Cu 4s, Cu 2p, and Cu 3d orbitals. When Cu 2+ adsorbed on the specularite (0 0 1) surface (Figure 5a), the PDOS of the Cu atom near the Fermi level was contributed by the 4s, 2p, and 3d orbitals, in which the contributions of Cu 3d and 4s orbitals were strong, and that played an important role in the reactivity of Cu 2+ adsorbed on the surface of specularite. Combined with the PDOS of Fe1 and O1 atoms on the surface of specularite (Figures 3b and 5a), it can be observed that the PDOS of the Cu 3d orbital peak at −1.3 eV and the Cu 2p orbital at 5 eV overlapped with the 2p orbital of the O1 atom on the specularite surface, indicating that Cu 2+ mainly interacted with the O atoms on the surface of the specularite.
inerals 2021, 11, x FOR PEER REVIEW 10 of 16 in Figure 5. As shown in Figure 5, the PDOS of Cu atoms after adsorption on the specularite surface was composed of Cu 4s, Cu 2p, and Cu 3d orbitals. When Cu 2+ adsorbed on the specularite (0 0 1) surface (Figure 5a), the PDOS of the Cu atom near the Fermi level was contributed by the 4s, 2p, and 3d orbitals, in which the contributions of Cu 3d and 4s orbitals were strong, and that played an important role in the reactivity of Cu 2+ adsorbed on the surface of specularite. Combined with the PDOS of Fe1 and O1 atoms on the surface of specularite (Figures 3b and 5a), it can be observed that the PDOS of the Cu 3d orbital peak at -1.3 eV and the Cu 2p orbital at 5 eV overlapped with the 2p orbital of the O1 atom on the specularite surface, indicating that Cu 2+ mainly interacted with the O atoms on the surface of the specularite. When Cu(OH) + adsorbed on the specularite (0 0 1) surface (Figure 5b), the PDOS of the Cu 4s orbital peak near the Fermi level became weaker and shifted to the right, and the PDOS of Cu 4s orbital at 1.96 eV overlapped with that of the OI atom of Cu(OH) + . Combined with the PDOS of O1 atom on the specularite surface (Figure 4c), it was found that the 4s orbital of the Cu atom overlapped with the 2s orbital of O atom on the specularite surface, indicating that the Cu atom of Cu(OH) + may have interacted with the O atoms on the specularite surface. At the same time, by comparing the PDOS of OI atoms of Cu (OH) + with that of Fe1 atoms on the surface of specularite (Figures 3c and 5b), it can be seen that the new peaks appeared at −20 eV, which attributed to the Fe 4s and 3d orbital and overlapped with the OI 2p orbital, indicating that the OI atoms of Cu(OH) + interacted with the Fe atoms on the surface of the specularite, which further confirmed that the appearance of new 4s orbital peaks of Fe atoms on the surface of specularite at -20 eV was caused by the adsorption of Cu(OH) + . When Cu(OH) + adsorbed on the specularite (0 0 1) surface (Figure 5b), the PDOS of the Cu 4s orbital peak near the Fermi level became weaker and shifted to the right, and the PDOS of Cu 4s orbital at 1.96 eV overlapped with that of the OI atom of Cu(OH) + . Combined with the PDOS of O1 atom on the specularite surface (Figure 4c), it was found that the 4s orbital of the Cu atom overlapped with the 2s orbital of O atom on the specularite surface, indicating that the Cu atom of Cu(OH) + may have interacted with the O atoms on the specularite surface. At the same time, by comparing the PDOS of OI atoms of Cu (OH) + with that of Fe1 atoms on the surface of specularite (Figures 3c and 5b), it can be seen that the new peaks appeared at −20 eV, which attributed to the Fe 4s and 3d orbital and overlapped with the OI 2p orbital, indicating that the OI atoms of Cu(OH) + interacted with the Fe atoms on the surface of the specularite, which further confirmed that the appearance of new 4s orbital peaks of Fe atoms on the surface of specularite at -20 eV was caused by the adsorption of Cu(OH) + .
Similarly, when Cu(OH) 2 adsorbed on the specularite (0 0 1) surface (Figure 5c), the PDOS of the Cu 4s orbital near the Fermi level disappeared, indicating that the contribution of the Cu 4s orbital to the activity of the Cu atom of Cu(OH) 2 was reduced, and the activity of Cu atom was mainly contributed by the Cu 3d orbital. The PDOS of Cu atoms overlapped with two O atoms (OI and OII) of Cu(OH) 2 , and there was no obvious overlap compared with the PDOS of O atoms on the surface of specularite, indicating that Cu atoms did not interact with the O atoms on the surface of specularite. By comparing the PDOS of the OI atom with that of the Fe1 atom on the surface (Figures 3d and 5c), it is obvious that the two new Fe 4s orbital peaks and a new Fe 3d orbital peak of the Fe1 atom at -20 eV overlapped with the O 2s orbital of the OI atom, indicating that Cu(OH) 2 was mainly absorbed on the specularite surface through the OI atom of -OH interacting with the surface Fe atoms. This further confirmed that the appearance of two new 4s orbital peaks and a new 3d orbital peak of Fe atom on the specularite surface at -20 eV was caused by the adsorption of Cu(OH) 2 .
In summary, the adsorption of Cu species on the surface of specularite was different. Cu 2+ may be adsorbed on the surface of specularite through the Cu atom directly interacting with O atoms to form Cu-O complexes, while Cu(OH) + and Cu(OH) 2 may be adsorbed on the surface of specularite through the interaction between OI (OII) atoms in -OH and Fe atoms on the surface of specularite to form Cu-O-Fe complexes.

Interatomic Charge Transfer Analysis of Interaction between Cu Species and Specularite (0 0 1) Surface
Mulliken charge populations of bonding atoms before and after Cu species adsorption are shown in Table 4. The results show that the adsorption of adsorbates on the surface of specularite (0 0 1) led to a change in the charge of the bonding atoms and that the variation of them was in regard to Cu species. In the absence of an adsorbate on the surface, the charge of the Fe1 atom exhibited 0.86 e, in which Fe atoms lost electrons in the 4s and 2p orbitals and gained electrons in the 3d orbital; the charge of the O1 atom was -0.59 e, in which the O lost electrons in the 2s orbital and gained electrons in the 2p orbital, indicating that electrons were transferred from Fe atoms to O atoms to form Fe-O bonds. When Cu 2+ adsorbed on the surface of specularite, the charge of Fe1 atom decreased from 0.86 to 0.68 e, with a decrease of 0.18 e; the charge of O1 atoms decreased from −0.59 to -0.62 e, with a decrease of 0.03 e. The electrons were obtained mainly in the O 2p orbitals, while the charge of the Cu atom was 0.50 e; the electrons were mainly lost in the Cu 4s orbitals compared with the charge before adsorption. Combining the above charge analysis between atoms, it is clear that the charges in the Cu-O1 bond formed by the adsorption of Cu 2+ on the surface of specularite were mainly transferred from the 4s orbital of the Cu atom to the 2p orbital of the O1 atom.
When CuOH + adsorbed on the surface of specularite, the charge of surface Fe1 atom increased by 0.09 e from 0.86 to 0.95 e, where the main contributions of lost electrons were Fe 4s and Fe 2p orbitals. The charge of O1 atoms decreased by 0.05 e from -0.59 to -0.64 e, with the gained electrons mainly in the O 2p orbitals, while the charge of the Cu atom increased from 0.48 to 0.50 e, with the loss of electrons mainly in the Cu 4s orbital. In addition, the charge of the OI atom of Cu(OH) + increased from -0.93 to -0.83 e, with the gain of electrons mainly in the OI 2p orbital. Combined with the above charge analysis between atoms, it is observed that the charges in the Cu-O1 bond formed after the adsorption of Cu(OH) + were mainly transferred from the Cu 4s orbital to the O1 2p orbital and that the charges in the Fe1-OI bond formed were mainly transferred from the 4s and 2p orbitals of the Fe1 atom to the 2p orbital of the OI atom. When Cu(OH) 2 adsorbed on the surface of specularite, the charge of surface Fe1 atoms increased from 0.86 to 0.95 e, with an increase of 0.09 e, in which the main contributions of lost electrons were Fe 4s and Fe 2p orbitals. The charge of O1 atoms remained essentially unchanged, indicating that the adsorption of Cu(OH) 2 had no significant effect on the charge of O1 atoms on the surface, which further confirms that the surface O1 atoms were not participating in the adsorption of Cu(OH) 2 on the specularite. The charge of the Cu atom decreased from 0.84 to 0.67 e, and the orbital lost electrons were mainly in Cu 4s, while the charges of OI and OII atoms increased from -0.87 and -0.88 to -0.81 and -0.83 e, with an increase of 0.06 e and 0.05 e, respectively, and the orbital gained electrons mainly in OI(OII) 2p. Combining the above charges between the atoms, it is clear that the charges in the Fe1-OI(OII) bond formed after the adsorption of Cu(OH) 2 were mainly transferred from the 4s and 2p orbitals of the Fe1 atom to the 2p orbitals of the OI(OII) atom. To further investigate the interaction between Cu components and the specularite surface, an electron density of different adsorbents adsorbed on the surface of specularite is shown in Figure 6, where different charge density is represented by different colors. Where the color goes from red to blue represents a gradual decrease in the ability of the atoms to gain electrons. The results in Figure 6 are consistent with the charge transfer results described above.

Analysis of Bond Properties of Cu Species Adsorbed on the Specularite Surface
The Mulliken bond population can reflect the strength of ionicity and covalency. The larger the bond population, the stronger the covalency, and the smaller the bond population, the stronger the ionicity [33,38,39]. In order to further understand the bonding properties between atoms in the specularite surface and Cu components, we compared the Mulliken bond populations of different Cu components adsorbed on the surface of specularite (0 0 1), as shown in Table 5.

Analysis of Bond Properties of Cu Species Adsorbed on the Specularite Surface
The Mulliken bond population can reflect the strength of ionicity and covalency. larger the bond population, the stronger the covalency, and the smaller the bond pop tion, the stronger the ionicity [34,39,40]. In order to further understand the bonding p erties between atoms in the specularite surface and Cu components, we compared Mulliken bond populations of different Cu components adsorbed on the surface of s ularite (0 0 1), as shown in Table 5. When Cu 2+ adsorbed on the specularite surface, the bond population of Cu-O1 0.14, which indicates that Cu-O had stronger ionicity and weaker covalency. W Cu(OH) + adsorbed on the specularite surface, the bond populations of Cu-O1 and Fe1 were 0.17 and 0.33, respectively, indicating that Cu-O had stronger ionicity, while F had stronger covalency. When Cu(OH)2 adsorbed on the surface of specularite, the b population of Fe1-OI(OII) was 0.30. It shows that Fe-O had stronger ionicity and we covalency. By comparing the Cu-O and Fe-O of the three Cu components on the sur  When Cu 2+ adsorbed on the specularite surface, the bond population of Cu-O1 was 0.14, which indicates that Cu-O had stronger ionicity and weaker covalency. When Cu(OH) + adsorbed on the specularite surface, the bond populations of Cu-O1 and Fe1-OI were 0.17 and 0.33, respectively, indicating that Cu-O had stronger ionicity, while Fe-O had stronger covalency. When Cu(OH) 2 adsorbed on the surface of specularite, the bond population of Fe1-OI(OII) was 0.30. It shows that Fe-O had stronger ionicity and weaker covalency. By comparing the Cu-O and Fe-O of the three Cu components on the surface of specularite (0 0 1), it can be seen that the bond population of Cu-O was smaller than that of Fe-O, indicating that the Cu-O was more ionic and Fe-O was more covalent.

Conclusions
In this work, the effect of Cu species adsorption on the crystalline structure and properties of specularite (0 0 1) was investigated by DFT calculations. Additionally, the activation mechanism of Cu 2+ on the flotation of specularite was discussed based on